Report

1 Anisotropic Elasticity Objective Linear Ferromagnets Non-linear properties Electric. Conduct. 27-750 Texture, Microstructure & Anisotropy A.D. Rollett Tensors Elasticity Symmetry Last revised: 7th Feb. ‘14 2 Bibliography • Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry • • • • • R.E. Newnham, Properties of Materials: Anisotropy, Symmetry, Structure, Oxford University Press, 2004, 620.112 N55P. Nye, J. F. (1957). Physical Properties of Crystals. Oxford, Clarendon Press. Kocks, U. F., C. Tomé and R. Wenk (1998). Texture and Anisotropy, Cambridge University Press, Cambridge, UK. Chapter 7. T. Courtney, Mechanical Behavior of Materials, McGraw-Hill, 0-07-013265-8, 620.11292 C86M. Reid, C. N. (1973). Deformation Geometry for Materials Scientists. Oxford, UK, Pergamon. Newey, C. and G. Weaver (1991). Materials Principles and Practice. Oxford, England, Butterworth-Heinemann. 3 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Notation F R P j E D d C S Stimulus (field) Response Property electric current electric field electric polarization Strain Stress (or conductivity) Resistivity piezoelectric tensor elastic stiffness elastic compliance a transformation matrix W work done (energy) dW work increment I identity matrix O symmetry operator (matrix) Y Young’s modulus Kronecker delta e axis (unit) vector T tensor direction cosine 4 Objective • The objective of this lecture is to provide a mathematical framework for the description of properties, especially when they vary with Objective direction. Linear • A basic property that occurs in almost applications is elasticity. Although elastic response is linear for all practical purposes, it is often Ferroanisotropic (composites, textured polycrystals etc.). magnets Non-linear • Why do we care about elastic anisotropy? In composites, especially properties fibre composites, it is easy to design in substantial anisotropy by varying the lay-up of the fibres. See, for example: Electric. http://www.jwave.vt.edu/crcd/kriz/lectures/Geom_3.html Conduct. Tensors • Geologists are very familiar with elastic anisotropy and exploit it for understanding seismic results. Elasticity Symmetry 5 In Class Questions 1. Why is plastic yielding a non-linear property, in contrast to elastic deformation? Objective 2. What is the definition of a tensor? 3. Why is stress is 2nd-rank tensor? Linear 4. Why is elastic stiffness a 4th-rank tensor? Ferromagnets 5. What is “matrix notation” (in the context of elasticity)? What are the relationships between tensor and matrix coefficients for Non-linear 6. stress? Strain? Stiffness? Compliance? properties Electric. 7. Why do we need factors of 2 and 4 in some of these conversion factors? Conduct. 8. How do we use crystal symmetry to decrease the number of coefficients needed to describe stiffness and compliance? Tensors 9. How many independent coefficients are needed for stiffness (and Elasticity compliance) in cubic crystals? In isotropic materials? Symmetry 10. How do we express the directional dependence of Young’s modulus? 11. What is Zener’s anisotropy factor? 6 Anisotropy: Practical Applications Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry • The practical applications of anisotropy of composites, especially fiber-reinforced composites are numerous. • The stiffness of fiber composites varies tremendously with direction. Torsional rigidity is very important in car bodies, boats, aeroplanes etc. • Even in monolithic polymers (e.g. drawn polyethylene) there exists large anisotropy because of the alignment of the long-chain molecules. 7 Application example: quartz oscillators • Piezoelectric quartz crystals are commonly used for frequency control in watches and clocks. Despite having small values of the piezoelectric coefficients, quartz has positive aspects of low losses Objective and the availability of orientations with negligible temperature sensitivity. The property of piezoelectricity relates strain to electric Linear field, or polarization to stress. Ferroij = dijkEk magnets • Non-linear • PZT, lead zirconium titanate PbZr1-xTixO3, is another commonly used properties piezoelectric material. Electric. Conduct. Tensors Elasticity Symmetry 8 Objective Linear Ferromagnets Non-linear properties Piezoelectric Devices Examinable • The property of piezoelectricity relates strain to electric field, or polarization to stress. ij = dijkEk • PZT, lead zirconium titanate PbZr1-xTixO3, is another commonly used piezoelectric material. Note: Newnham consistently uses vector-matrix notation, rather than tensor notation. We will explain how this works later on. Electric. Conduct. Tensors Elasticity Symmetry [Newnham] 9 Piezoelectric Crystals • • Objective Linear Ferromagnets • Non-linear properties Electric. Conduct. • Tensors Elasticity Symmetry How is it that crystals can be piezoelectric? The answer is that the bonding must be ionic to some degree (i.e. there is a net charge on the different elements) and the arrangement of the atoms must be non-centrosymmetric. PZT is a standard piezoelectric material. It has Pb atoms at the cell corners (a~4Å), O on face centers, and a Ti or Zr atom near the body center. Below a certain temperature (Curie T), the cell transforms from cubic (high T) to tetragonal (low T). Applying stress distorts the cell, which changes the electric displacement in different ways (see figure). Although we can understand the effect at the single crystal level, real devices (e.g. sonar transducers) are polycrystalline. The operation is much complicated than discussed here, and involves “poling” to maximize the response, which in turns involves motion of domain walls. [Newnham] 10 Mathematical Descriptions • Mathematical descriptions of properties are available. • Mathematics, or a type of mathematics provides a quantitative framework. It is always necessary, however, Objective to make a correspondence between mathematical Linear variables and physical quantities. Ferromagnets • In group theory one might say that there is a set of Non-linear mathematical operations & parameters, and a set of properties physical quantities and processes: if the mathematics is a Electric. good description, then the two sets are isomorphous. Conduct. Tensors • This lecture makes extensive use of tensors. A tensor is a quantity that can be transformed from one set of axes to Elasticity another via the tensor transformation rule (next slide). Symmetry 11 Objective Linear Ferromagnets Tensor: definition, contd. • In order for a quantity to “qualify” as a tensor it has to obey the axis transformation rule, as discussed in the previous slides. • The transformation rule defines relationships between transformed and untransformed tensors of various ranks. Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Vector: 2nd rank 3rd rank 4th rank V’i = aijVj T’ij = aikajlTkl T’ijk = ailajmaknTlmn T’ijkl = aimajnakoalpTmnop This rule is a critical piece of information, which you must know how to use. 12 Non-Linear properties, example • Another important example of non-linear anisotropic properties is plasticity, i.e. the irreversible deformation of solids. • A typical description of the response at plastic yield Objective (what happens when you load a material to its yield stress) Linear is elastic-perfectly plastic. In other words, the material responds Ferroelastically until the yield stress is magnets reached, at which point the stress Non-linear remains constant (strain rate properties unlimited). Electric. Conduct. Tensors Elasticity Symmetry • A more realistic description is a power-law with a large exponent, n~50. The stress is scaled by the crss, and be expressed as either shear stressshear strain rate [graph], or tensile stress-tensile strain [equation]. æ s ö ÷ e˙ = ç è s yield ø [Kocks] n 13 Objective Linear properties • Certain properties, such as elasticity in most cases, are linear which means that we can simplify even further to obtain Linear Ferromagnets Non-linear or if R0 = 0, properties Electric. Conduct. Tensors Elasticity Symmetry e.g. elasticity: R = R0 + PF R = PF. stiffness =C In tension, C Young’s modulus, Y or E. 14 Elasticity • Elasticity: example of a property that requires tensors to describe it fully. Objective • Even in cubic metals, a crystal is quite anisotropic. The Linear [111] in many cubic metals is stiffer than the [100] Ferrodirection. magnets Non-linear • Even in cubic materials, 3 numbers/coefficients/moduli properties are required to describe elastic properties; isotropic Electric. materials only require 2. Conduct. • Familiarity with Miller indices, suffix notation, Einstein Tensors convention, Kronecker delta, permutation tensor, and Elasticity tensors is assumed. Symmetry 15 Elastic Anisotropy: 1 • First we restate the linear elastic relations for the properties Compliance, written S, and Stiffness, Objective written C (admittedly not very logical choice of Linear notation), which connect stress, , and strain, . FerroWe write it first in vector-tensor notation with “:” magnets signifying inner product (i.e. add up terms that Non-linear properties have a common suffix or index in them): Electric. = C: Conduct. = S: Tensors Elasticity • In component form (with suffices), Symmetry ij = Cijklkl ij = Sijklkl 16 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Elastic Anisotropy: 2 The definitions of the stress and strain tensors mean that they are both symmetric (second rank) tensors. Therefore we can see that 23 = S231111 32 = S321111 = 23 which means that, S2311 = S3211 and in general, Sijkl = Sjikl We will see later on that this reduces considerably the number of different coefficients needed. 17 Stiffness in sample coords. • Consider how to express the elastic properties of a single crystal in the sample coordinates. In this case we need to Objective rotate the (4th rank) tensor stiffness from crystal Linear coordinates to sample coordinates using the orientation Ferro(matrix), a : magnets cijkl' = aimajnakoalpcmnop Non-linear properties • Note how the transformation matrix appears four times Electric. because we are transforming a 4th rank tensor! Conduct. • The axis transformation matrix, a, is sometimes also Tensors written as l, also as the transpose of the orientation Elasticity matrix gT. Symmetry 18 Young’s modulus from compliance • Young's modulus as a function of direction can be obtained from the compliance tensor as: Objective E=1/s'1111 Linear Using compliances and a stress boundary Ferromagnets condition (only 110) is most straightforward. Non-linear To obtain s'1111, we simply apply the same properties transformation rule, Electric. Conduct. Tensors Elasticity Symmetry s'ijkl = aim ajn ako alpsmnop 19 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry “Voigt” or “matrix” notation • It is useful to re-express the three quantities involved in a simpler format. The stress and strain tensors are vectorized, i.e. converted into a 1x6 notation and the elastic tensors are reduced to 6x6 matrices. æ s1 1 s 1 2 s 1 3ö æ s 1 s 6 s 5ö ç s 2 1 s 2 2 s 2 3÷ ¬¾®ç s 6 s 2 s 4 ÷ ç ÷ ç ÷ è s 3 1 s 3 2 s 3 3ø ès 5 s 4 s 3ø ¬¾®(s 1 ,s 2 , s 3 , s 4 ,s 5 ,s 6 ) 20 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry “matrix notation”, contd. • Similarly for strain: æ e1 æ e1 1 e1 2 e1 3ö ç e 2 1 e 2 2 e 2 3÷ ¬¾®ç 1 e 6 ç ÷ ç 21 è e 3 1 e 3 2 e 3 3ø è 2 e5 e6 e2 1 e 2 4 1 2 e5 ö e4 ÷ ÷ e3 ø 1 2 1 2 ¬¾®(e 1 ,e 2 , e 3 , e 4 , e 5 , e 6 ) The particular definition of shear strain used in the reduced notation happens to correspond to that used in mechanical engineering such that 4 is the change in angle between direction 2 and direction 3 due to deformation. 21 Work conjugacy, matrix inversion Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry • The more important consideration is that the reason for the factors of two is so that work conjugacy is maintained. dW = :d = ij : dij = k • dk Also we can combine the expressions = C and = S to give: = CS, which shows: I = CS, or, C = S-1 22 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Tensor conversions: stiffness • Lastly we need a way to convert the tensor coefficients of stiffness and compliance to the matrix coefficients. For stiffness, it is very simple because one substitutes values according to the following table, such that matrixC11 = tensorC1111 for example. Tensor Matrix 11 1 22 2 33 3 23 4 32 4 13 5 31 5 12 6 21 6 23 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Stiffness Matrix éC1 1 êC 21 ê êC3 1 C =ê C4 1 ê êC5 1 êC ë 61 C1 2 C1 3 C1 4 C2 2 C2 3 C2 4 C 3 2 C3 3 C 3 4 C4 2 C4 3 C4 4 C5 2 C5 3 C5 4 C6 2 C6 3 C6 4 C1 5 C1 6 ù ú C 2 5 C2 6 ú C 3 5 C3 6 ú C 4 5 C 4 6ú ú C 5 5 C5 6 ú ú C 6 5 C6 6 û 24 Tensor conversions: compliance • For compliance some factors of two are required and so the rule becomes: Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry pSijkl = Smn p =1 p=2 p=4 m.AND.n Î[1,2, 3] m .XOR.n Î[1, 2, 3] m.AND.n Î[ 4,5,6 ] 25 Relationships between coefficients: C in terms of S Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Some additional useful relations between coefficients for cubic materials are as follows. Symmetrical relationships exist for compliances in terms of stiffnesses (next slide). C11 = (S11+S12)/{(S11-S12)(S11+2S12)} C12 = -S12/{(S11-S12)(S11+2S12)} C44 = 1/S44. 26 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry S in terms of C The relationships for S in terms of C are symmetrical to those for stiffnesses in terms of compliances (a simple exercise in algebra). S11 = (C11+C12)/{(C11-C12)(C11+2C12)} S12 = -C12/{(C11-C12)(C11+2C12)} S44 = 1/C44. 27 Neumann's Principle • A fundamental natural law: Neumann's Principle: Objective the symmetry elements of any physical property Linear of a crystal must include the symmetry elements Ferroof the point group of the crystal. The property magnets may have additional symmetry elements to those Non-linear properties of the crystal (point group) symmetry. There are Electric. 32 crystal classes for the point group symmetry. Conduct. Tensors • F.E. Neumann 1885. Elasticity Symmetry 28 Neumann, extended • If a crystal has a defect structure such as a dislocation network that is arranged in a non-uniform way then the Objective symmetry of certain properties may be reduced from the Linear crystal symmetry. In principle, a finite elastic strain in one Ferrodirection decreases the symmetry of a cubic crystal to magnets Non-linear tetragonal or less. Therefore the modified version of properties Neumann's Principle: the symmetry elements of any Electric. physical property of a crystal must include the symmetry Conduct. elements that are common to the point group of the Tensors crystal and the defect structure contained within the Elasticity crystal. Symmetry 29 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Effect of crystal symmetry • Consider an active rotation of the crystal, where O is the symmetry operator. Since the crystal is indistinguishable (looks the same) after applying the symmetry operator, the result before, R(1), and the result after, R(2), must be identical: ü R = PF ï (2) T ï R = OPO F ý = (1) (2 ) ï R ¬ ¾ ® R ïþ (1) The two results are indistinguishable and therefore equal. It is essential, however, to express the property and the operator in the same (crystal) reference frame. 30 Symmetry, properties, contd. • Objective Linear Ferromagnets • Non-linear properties • Electric. Conduct. • Tensors Elasticity Symmetry • Expressed mathematically, we can rotate, e.g. a second rank property tensor thus: P' = OPOT = P , or, in coefficient notation, P’ij = OikOilPkl where O is a symmetry operator. Since the rotated (property) tensor, P’, must be the same as the original tensor, P, then we can equate coefficients: P’ij = Pij If we find, for example, that P’21 = -P21,then the only value of P21 that satisfies this equality is P21 = 0. Remember that you must express the property with respect to a particular set of axes in order to use the coefficient form. In everything related to single crystals, always use the crystal axes as the reference frame! Homework question: based on cubic crystal symmetry, work out why a second rank tensor property can only have one independent coefficient. 31 Effect of symmetry on stiffness matrix • Why do we need to look at the effect of symmetry? For a cubic material, only 3 independent coefficients are needed Objective as opposed to the 81 coefficients in a 4th rank tensor. Linear The reason for this is the symmetry of the material. Ferromagnets • What does symmetry mean? Fundamentally, if you pick up a crystal, rotate [mirror] it and put it back down, then a Non-linear properties symmetry operation [rotation, mirror] is such that you Electric. cannot tell that anything happened. Conduct. • From a mathematical point of view, this means that the Tensors property (its coefficients) does not change. For example, Elasticity if the symmetry operator changes the sign of a coefficient, Symmetry then it must be equal to zero. 32 2nd Rank Tensor Properties & Symmetry Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry • The table from Nye shows the number of independent, non-zero coefficients allowed in a 2nd rank tensor according to the crystal symmetry class. 33 Effect of symmetry on stiffness matrix Objective Linear • Following Reid, p.66 et seq.: Apply a 90° rotation about the crystal-z axis (axis 3), C’ijkl = OimOjnOkoOlpCmnop: æ 0 -1 0ö C’ = C ç ÷ z O4 Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry é C22 ê ê C21 ê ê C23 C¢ = ê ê C25 ê-C24 ê êë-C26 C21 C11 C13 C15 C23 C13 C33 C35 C25 C15 C35 C55 -C24 -C14 -C34 -C54 -C14 -C16 -C34 -C36 -C54 -C56 C44 C46 = ç1 ç è0 -C26 ù ú -C16 ú ú -C36 ú -C56 úú C46 ú ú C66 úû 0 0 0÷ ÷ 1ø 34 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Effect of symmetry, 2 • Using P’ = P, we can equate coefficients and find that: C11=C22, C13=C23, C44=C35, C16=-C26, C14=C15 = C24 = C25 = C34 = C35 = C36 = C45 = C46 = C56 = 0. é ê ê ê C¢ = ê ê ê ê ê ë C11 C12 C13 0 0 C12 C11 C13 0 0 C13 C13 C33 0 0 0 0 0 C44 0 0 0 0 0 C44 C16 -C16 0 0 C46 C16 ù ú -C16 ú ú 0 ú 0 ú ú C46 ú C66 úû 35 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Effect of symmetry, 3 • Thus by repeated applications of the symmetry operators, one can demonstrate (for cubic crystal symmetry) that one can reduce the 81 coefficients down to only 3 independent quantities. These become two in the case of isotropy. éC11 ê êC12 ê êC12 ê 0 ê ê 0 ê êë 0 C12 C12 0 0 0 ù ú C11 C12 0 0 0 ú ú C12 C11 0 0 0 ú 0 0 C44 0 0 úú 0 0 0 C44 0 ú ú 0 0 0 0 C44 úû 36 Cubic crystals: anisotropy factor Objective Linear Ferromagnets Non-linear • If one applies the symmetry elements of the cubic system, it turns out that only three independent coefficients remain: C11, C12 and C44, (similar set for compliance). From these three, a useful combination of the first two is properties Electric. Conduct. C' = (C11 - C12)/2 Tensors Elasticity Symmetry • See Nye, Physical Properties of Crystals 37 Zener’s anisotropy factor • C' = (C11 - C12)/2 turns out to be the stiffness associated with a shear in a <110> direction on a Objective plane. In certain martensitic transformations, this Linear modulus can approach zero which corresponds to Ferromagnets a structural instability. Zener proposed a Non-linear measure of elastic anisotropy based on the ratio properties C44/C'. This turns out to be a useful criterion for Electric. Conduct. identifying materials that are elastically Tensors anisotropic. Elasticity Symmetry 38 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Rotated compliance (matrix) • Given an orientation aij, we transform the compliance tensor, using cubic point group symmetry, and find that: ( S1¢ 1 = S1 1 a141 + a142 + a143 ( + 2 2 2S1 2 a1 2a1 3 + 2 2 S4 4 a1 2a1 3 + ( + ) 2 2 a1 1a1 2 2 2 a1 1a1 2 + + ) 2 2 a1 1a1 3 2 2 a1 1a1 3 ) 39 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Rotated compliance (matrix) • This can be further simplified with the aid of the standard relations between the direction cosines, aikajk = 1 for i=j; aikajk = 0 for ij, (aikajk = ij) to read as follows. s11¢ = s11 æ s44 ö 2 2 2 2 2 2 2ç s11 - s12 - ÷{a1 a 2 + a 2a 3 + a 3a1 } è 2ø • By definition, the Young’s modulus in any direction is given by the reciprocal of the compliance, E = 1/S’11. 40 Anisotropy in cubic materials • Thus the second term on the RHS is zero for <100> directions and, for C44/C'>1, a maximum in <111> Objective directions (conversely Linear Material C /C' E /E a minimum for C44/C'<1). Cu 3.21 2.87 FerroNi 2.45 2.18 The following table shows magnets A1 1.22 1.19 that most cubic metals have Fe 2.41 2.15 Non-linear Ta 1.57 1.50 positive values of Zener's properties W (2000K) 1.23 1.35 W (R.T.) 1.01 1.01 coefficient so that <100> Electric. V 0.78 0.72 Conduct. is soft and <111> is hard, Nb 0.55 0.57 b-CuZn 18.68 8.21 Tensors with the exceptions of V spinel 2.43 2.13 MgO 1.49 1.37 and NaCl. Elasticity 44 Symmetry NaC1 0.69 111 100 0.74 41 Stiffness coefficients, cubics Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry [Courtney] 42 Anisotropy in terms of moduli • Another way to write the above equation is to insert the values for the Young's modulus in the Objective soft and hard directions, assuming that the Linear <100> are the most compliant direction(s). Ferromagnets (Courtney uses , b, and g in place of my 1, 2, Non-linear and 3.) The advantage of this formula is that properties moduli in specific directions can be used directly. Electric. Conduct. Tensors Elasticity Symmetry ì 1 1 1 1 ü 2 2 2 2 2 2 = - 3í a a + a a + a ý( 1 2 2 3 3 a1 ) Euvw E100 î E100 E111þ 43 Example Problem Objective Linear Ferromagnets [Courtney] Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Should be E<111>= 18.89 44 Alternate Vectorization Objective Linear Ferromagnets Non-linear properties An alternate vectorization, discussed by Tomé on p287 of the Kocks et al. Electric. textbook, is to use the above set of eigentensors. For both stress and strain, Conduct. one can matrix multiply each eigentensor into the stress/strain tensor in turn and obtain the coefficient of the corresponding stress/strain vector. Work Tensors conjugacy is still satisfied. The first two eigentensors represent shears in the Elasticity {110} planes; the next three are simple shears on {110}<110> systems, and the Symmetry last (6th) is the hydrostatic component. The same vectorization can be used for plastic anisotropy, except in this case, the sixth, hydrostatic component is (generally) ignored. 45 Summary • We have covered the following topics: Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry – – – – – Linear properties Non-linear properties Examples of properties Tensors, vectors, scalars, tensor transformation law. Elasticity, as example as of higher order property, also as example as how to apply (crystal) symmetry. 46 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Supplemental Slides • The following slides contain some useful material for those who are not familiar with all the detailed mathematical methods of matrices, transformation of axes, tensors etc. 47 Einstein Convention • The Einstein Convention, or summation rule for suffixes looks like this: Objective Ai = Bij Cj Linear where “i” and “j” both are integer indexes whose Ferroth” component range is {1,2,3}. So, to find each “i magnets of A on the LHS, we sum up over the repeated Non-linear properties index, “j”, on the RHS: Electric. A1 = B11C1 + B12C2 + B13C3 Conduct. A2 = B21C1 + B22C2 + B23C3 Tensors Elasticity A3 = B31C1 + B32C2 + B33C3 Symmetry 48 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Matrix Multiplication • Take each row of the LH matrix in turn and multiply it into each column of the RH matrix. • In suffix notation, aij = bikckj éaa + bd + cg ê êda + e d + fg ê ëla + md + ng éa b ê = êd e ê ël m ab + be + cm ag + bf + cn ù ú db + ee + f m dg + ef + fn ú ú lb + me + nm lg + mf + nn û c ù éa ú ê f ú ´ êd ú ê n û ël b gù ú e fú ú m nû 49 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Properties of Rotation Matrix • The rotation matrix is an orthogonal matrix, meaning that any row is orthogonal to any other row (the dot products are zero). In physical terms, each row represents a unit vector that is the position of the corresponding (new) old axis in terms of the (old) new axes. • The same applies to columns: in suffix notation aijakj = ik, ajiajk = ik éa b ê êd e ê ël m cù ú fú ú nû ad+be+cf = 0 bc+ef+mn = 0 50 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Direction Cosines, contd. • That the set of direction cosines are not independent is evident from the following construction: eˆi¢ × eˆ¢j = aik a jl eˆk × eˆl = aik a jldkl = aik a jk = dij Thus, there are six relationships (i takes values from 1 to 3, and j takes values from 1 to 3) between the nine direction cosines, and therefore, as stated above, only three are independent, exactly as expected for a rotation. • Another way to look at a rotation: combine an axis (described by a unit vector with two parameters) and a rotation angle (one more parameter, for a total of 3). 51 Objective Orthogonal Matrices • Note that the direction cosines can be arranged into a 3x3 matrix, L, and therefore the relation above is equivalent to the expression T Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry LL = I where L T denotes the transpose of L. This relationship identifies L as an orthogonal matrix, which has the properties -1 L T =L det L = ±1 52 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Relationships • When both coordinate systems are right-handed, det(L)=+1 and L is a proper orthogonal matrix. The orthogonality of L also insures that, in addition to the relation above, the following holds: eˆ j = aij eˆi¢ Combining these relations leads to the following interrelationships between components of vectors in the two coordinate systems: v i = a jiv ¢j , v ¢j = a jiv i 53 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Transformation Law • These relations are called the laws of transformation for the components of vectors. They are a consequence of, and equivalent to, the parallelogram law for addition of vectors. That such is the case is evident when one considers the scalar product expressed in two coordinate systems: u × v = uiv i = a ji u¢j akiv ¢k = d jk u¢j v ¢k = u¢j v ¢j = u¢iv ¢i 54 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Invariants Thus, the transformation law as expressed preserves the lengths and the angles between vectors. Any function of the components of vectors which remains unchanged upon changing the coordinate system is called an invariant of the vectors from which the components are obtained. The derivations illustrate the fact that the scalar product is an invariant of and . Other examples of invariants include the vector product of two vectors and the triple scalar product of three vectors. The reader should note that the transformation law for vectors also applies to the components of points when they are referred to a common origin. u× v u v 55 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Orthogonality • A rotation matrix, L, is an orthogonal matrix, however, because each row is mutually orthogonal to the other two. aki akj = dij , aik a jk = dij • Equally, each column is orthogonal to the other two, which is apparent from the fact that each row/column contains the direction cosines of the new/old axes in terms of the old/new axes and we are working with [mutually perpendicular] Cartesian axes. 56 Anisotropy • • Objective • Linear Ferromagnets • Non-linear properties • Electric. Conduct. Tensors Elasticity Symmetry • • Anisotropy as a word simply means that something varies with direction. Anisotropy is from the Greek: aniso = different, varying; tropos = direction. Almost all crystalline materials are anisotropic; many materials are engineered to take advantage of their anisotropy (beer cans, turbine blades, microchips…) Older texts use trigonometric functions to describe anisotropy but tensors offer a general description with which it is much easier to perform calculations. For materials, what we know is that some properties are anisotropic. This means that several numbers, or coefficients, are needed to describe the property - one number is not sufficient. Elasticity is an important example of a property that, when examined in single crystals, is often highly anisotropic. In fact, the lower the crystal symmetry, the greater the anisotropy is likely to be. Nomenclature: in general, we need to use tensors to describe fields and properties. The simplest case of a tensor is a scalar which is all we need for isotropic properties. The next “level” of tensor is a vector, e.g. electric current. 57 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Scalars, Vectors, Tensors • Scalar:= quantity that requires only one number, e.g. density, mass, specific heat. Equivalent to a zero-rank tensor. • Vector:= quantity that has direction as well as magnitude, e.g. velocity, current, magnetization; requires 3 numbers or coefficients (in 3D). Equivalent to a first-rank tensor. • Tensor:= quantity that requires higher order descriptions but is the same, no matter what coordinate system is used to describe it, e.g. stress, strain, elastic modulus; requires 9 (or more, depending on rank) numbers or coefficients. 58 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Vector field, response • If we have a vector response, R, that we can write in component form, a vector field, F, that we can also write in component form, and a property, P, that we can write in matrix form (with nine coefficients) then the linearity of the property means that we can write the following (R0 = 0): Ri = PijFj • A scalar (e.g. pressure) can be called a zero-rank tensor. Elasticity Symmetry • A vector (e.g. electric current) is also known as a first-rank tensor. Tensors 59 Linear anisotropic property • This means that each component of the response is linearly related to each component of the field and that Objective the proportionality constant is the appropriate coefficient Linear in the matrix. Example: FerroR1 = P13F3, magnets which says that the first component of the response is Non-linear properties linearly related to the third field component through the Electric. property coefficient P13. Conduct. Tensors Elasticity x3 R1 F3 Symmetry x1 60 Example: electrical conductivity Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry • An example of such a linear anisotropic (second order tensor, discussed in later slides) property is the electrical conductivity of a material: • Field: Electric Field, E • Response: Current Density, J • Property: Conductivity, • Ji = ij Ej 61 Anisotropic electrical conductivity Objective • We can illustrate anisotropy with Nye’s example of electrical conductivity, : Linear Ferromagnets Non-linear properties O Electric. Conduct. Tensors Elasticity Symmetry Stimulus/ Field: E10, E2=E3=0 Response: j1=11E1, j2=21E1, j3=31E1, 62 Changing the Coordinate System • Many different choices are possible for the orthonormal base vectors and origin of the Cartesian coordinate system. A vector is an example Objective of an entity which is independent of the choice of coordinate system. Linear Its direction and magnitude must not change (and are, in fact, invariants), although its components will change with this choice. Ferromagnets • Why would we want to do something like this? For example, Non-linear although the properties are conveniently expressed in a crystal properties reference frame, experiments often place the crystals in a nonsymmetric position with respect to an experimental frame. Therefore Electric. Conduct. we need some way of converting the coefficients of the property into the experimental frame. Tensors Elasticity • Changing the coordinate system is also known as axis transformation. Symmetry 63 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Tensor: definition, contd. • In order for a quantity to “qualify” as a tensor it has to obey the axis transformation rule, as discussed in the previous slides. • The transformation rule defines relationships between transformed and untransformed tensors of various ranks. Vector: 2nd rank 3rd rank 4th rank V’i = aijVj T’ij = aikailTkl T’ijk = ailaimaknTlmn T’ijkl = aimainakoalpTmnop • This rule is a critical piece of information, which you must know how to use. 64 Motivation for Axis Transformation Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry • One motivation for axis transformations is the need to solve problems where the specimen shape (and the stimulus direction) does not align with the crystal axes. Consider what happens when you apply a force parallel to the sides of this specimen … [100] The direction parallel to the long edge does not line up with any simple, low index crystal direction. Therefore we have to find a way to transform the properties that we know for the material into the frame of the problem (or vice versa). Applied stress [110] Image of Pt surface from www.cup.uni-muenchen.de/pc/wintterlin/IMGs/pt10p3.jpg 65 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry New Axes • Consider a new orthonormal system consisting of righthanded base vectors: eˆ1¢, eˆ¢2 and eˆ¢3 These all have the same origin, o, associated with eˆ1¢, eˆ¢2 and eˆ¢3 • The vector v is clearly expressed equally well in either coordinate system: v = v ieˆi = v¢ieˆ¢i Note - same physical vector but different values of the components. • We need to find a relationship between the two sets of components for the vector. 66 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Anisotropy in Composites • The same methods developed here for describing the anisotropy of single crystals can be applied to composites. • Anisotropy is important in composites, not because of the intrinsic properties of the components but because of the arrangement of the components. • As an example, consider (a) a uniaxial composite (e.g. tennis racket handle) and (b) a flat panel cross-ply composite (e.g. wing surface). 67 Fiber Symmetry z Objective Linear Ferromagnets Non-linear properties Electric. Conduct. y Tensors Elasticity Symmetry x 68 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Fiber Symmetry • We will use the same matrix notation for stress, strain, stiffness and compliance as for single crystals. • The compliance matrix, s, has 5 independent coefficients. é s11 ê ê s12 ê s13 ê ê0 ê0 ê ë0 s12 s13 0 0 s11 s13 0 0 s13 s33 0 0 0 0 s44 0 0 0 0 s44 0 0 0 0 ù ú 0 ú ú 0 ú 0 ú ú 0 ú 2( s11 - s12 )û 0 69 Relationships • For a uniaxial stress along the z (3) direction, Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry s3 1 æ s zz ö E3 = = ç= ÷ e 3 s33 è e zz ø • This stress causes strain in the transverse plane: e11 = e22 = s1233. Therefore we can calculate Poisson’s ratio as: n13 e1 s13 æ exx ö = = ç= ÷ e3 s33 è ezz ø • Similarly, stresses applied perpendicular to z give rise to different moduli and Poisson’s ratios. E1 = s1 1 -s -s = , n 21 = 12 , n 31 = 13 e1 s11 s11 s11 70 Objective Linear Ferromagnets Relationships, contd. • Similarly the torsional modulus is related to shears involving the z axis, i.e. yz or xz shears: s44 = s55 = 1/G • Shear in the x-y plane (1-2 plane) is related to the Non-linear other compliance coefficients: properties s66 = 2(s11-s12) = 1/Gxy Electric. Conduct. Tensors Elasticity Symmetry 71 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Plates: Orthotropic Symmetry • Again, we use the same matrix notation for stress, strain, stiffness and compliance as for single crystals. • The compliance matrix, s, has 9 independent coefficients. • This corresponds to othorhombic sample symmetry: see the following slide with Table from Nye’s book. é s11 ê ê s12 ê s13 ê ê0 ê0 ê ë0 s12 s13 0 0 s22 s23 0 0 s23 s33 0 0 0 0 s44 0 0 0 0 s55 0 0 0 0 0ù ú 0ú 0ú ú 0ú 0ú ú s66 û 72 Plates: 0° and 90° plies • If the composite is a laminate composite with fibers laid in at 0° and 90° in equal thicknesses then the symmetry is higher because the x and y directions are equivalent. Objective • The compliance matrix, s, has 6 independent coefficients. Linear • This corresponds to (tetragonal) 4mm sample symmetry: see the Ferrofollowing slide with Table from Nye’s book. magnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry é s11 ê ê s12 ê s13 ê ê0 ê0 ê ë0 s12 s13 0 0 s11 s13 0 0 s13 s33 0 0 0 0 s44 0 0 0 0 s44 0 0 0 0 0ù ú 0ú 0ú ú 0ú 0ú ú s66 û 73 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Effect of Symmetry on the Elasticity Tensors, S, C 74 General Anisotropic Properties Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry • Many different properties of crystals can be described as tensors. • The rank of each tensor property depends, naturally, on the nature of the quantities related by the property. 75 Examples of Materials Properties as Tensors • Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry • Table 1 shows a series of tensors that are of importance for material science. The tensors are grouped by rank, and are also labeled (in the last column) by E (equilibrium property) or T (transport property). The number following this letter indicates the maximum number of independent, nonzero elements in the tensor, taking into account symmetries imposed by thermodynamics. The Field and Response columns contain the following symbols: ∆T = temperature difference, ∆S = entropy change, Ei = electric field components, Hi = magnetic field components, ij = mechanical strain, Di = electric displacement, Bi = magnetic induction, ij = mechanical stress, ∆bij = change of the impermeability tensor, ji = electrical current density, jT = temperature gradient, hi = heat flux, jc = concentration gradient, mi = mass flux, ai = antisymmetric part of resistivity tensor, si = symmetric part of resistivity tensor, ∆ij = change in the component ij of the resistivity tensor, li = direction cosines of wave direction in crystal, G = gyration constant, 76 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry 77 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Courtesy of Prof. M. De Graef 78 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Courtesy of Prof. M. De Graef Principal Effects Electrocaloric = pyroelectric Magnetocaloric = pyromagnetic Thermal expansion = piezocaloric Magnetoelectric and converse magnetoelectric Piezoelectric and converse piezoelectric Piezomagnetic and converse piezomagnetic 79 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Principal Effects 1st rank cross effects 2nd rank cross effects 3rd rank cross effects Courtesy of Prof. M. De Graef 80 Objective Linear Ferromagnets Non-linear properties General crystal symmetry shown above. Electric. Conduct. Tensors Elasticity Symmetry Courtesy of Prof. M. De Graef 81 Objective Linear Ferromagnets Non-linear properties Point group 4 Electric. Conduct. Tensors Elasticity Symmetry Courtesy of Prof. M. De Graef 82 Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry Point group m3m Note how many fewer independent coefficients there are! Note how the center of symmetry eliminates many of the properties, such as pyroelectricity Courtesy of Prof. M. De Graef 83 Homogeneity • Objective Linear Ferromagnets Non-linear properties Electric. Conduct. Tensors Elasticity Symmetry • Stimuli and responses of interest are, in general, not scalar quantities but tensors. Furthermore, some of the properties of interest, such as the plastic properties of a material, are far from linear at the scale of a polycrystal. Nonetheless, they can be treated as linear at a suitably local scale and then an averaging technique can be used to obtain the response of the polycrystal. The local or microscopic response is generally well understood but the validity of the averaging techniques is still controversial in many cases. Also, we will only discuss cases where a homogeneous response can be reasonably expected. There are many problems in which a non-homogeneous response to a homogeneous stimulus is of critical importance. Stress-corrosion cracking, for example, is a wildly non-linear, non-homogeneous response to an approximately uniform stimulus which depends on the mechanical and electro-chemical properties of the material.